#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/10/4001028.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001028
loop_
_publ_author_name
'Mizoguchi, Hiroshi'
'Ramirez, A. P.'
'Siegrist, T.'
'Zakharov, L. N.'
'Sleight, A. W.'
'Subramanian, M. A.'
_publ_section_title
;
 Possible Verwey-Type Transition in Pb3Rh7O15
;
_journal_issue                   11
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2300
_journal_paper_doi               10.1021/cm900697s
_journal_volume                  21
_journal_year                    2009
_chemical_formula_sum            'Bi0.96 O15 Pb2.04 Rh7'
_chemical_formula_weight         1583.66
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           193
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXLTL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            4
_cell_length_a                   10.351(5)
_cell_length_b                   10.351(5)
_cell_length_c                   13.152(13)
_cell_measurement_reflns_used    2437
_cell_measurement_temperature    268(2)
_cell_measurement_theta_max      27.87
_cell_measurement_theta_min      3.10
_cell_volume                     1220.4(15)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'Bruker SHELXTL'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      268(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector Bruker Apex'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0458
_diffrn_reflns_av_sigmaI/netI    0.0155
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9490
_diffrn_reflns_theta_full        27.49
_diffrn_reflns_theta_max         27.49
_diffrn_reflns_theta_min         2.27
_exptl_absorpt_coefficient_mu    51.116
_exptl_absorpt_correction_T_max  0.597
_exptl_absorpt_correction_T_min  0.294
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            dark-blue
_exptl_crystal_density_diffrn    8.620
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cut-block
_exptl_crystal_F_000             2728
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_refine_diff_density_max         1.497
_refine_diff_density_min         -1.587
_refine_diff_density_rms         0.277
_refine_ls_extinction_coef       0.00015(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.276
_refine_ls_matrix_type           full
_refine_ls_number_parameters     51
_refine_ls_number_reflns         544
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.276
_refine_ls_R_factor_all          0.0228
_refine_ls_R_factor_gt           0.0212
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0218P)²+9.5014P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0487
_refine_ls_wR_factor_ref         0.0504
_reflns_number_gt                528
_reflns_number_total             544
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm900697s_si_002.cif
_cod_data_source_block           mrt16
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        1220.3(14)
_cod_original_sg_symbol_H-M      P6(3)/mcm
_cod_database_code               4001028
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'-y, -x, -z'
'-x+y, y, -z'
'x, x-y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'y, x, z'
'x-y, -y, z'
'-x, -x+y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Pb1 Pb 1.0000 0.39648(6) 0.2500 0.01580(18) Uani 0.68 4 d SP
Bi1 Bi 1.0000 0.39648(6) 0.2500 0.01580(18) Uani 0.32 4 d SP
Pb2 Pb 0.73608(6) 0.0000 0.2500 0.01242(17) Uani 0.68 4 d SP
Bi2 Bi 0.73608(6) 0.0000 0.2500 0.01242(17) Uani 0.32 4 d SP
Rh1 Rh 0.6667 0.3333 0.14824(7) 0.0037(2) Uani 1 3 d S
Rh2 Rh 0.66407(8) -0.16797(4) 0.0000 0.0049(2) Uani 1 2 d S
Rh3 Rh 1.0000 0.0000 0.0000 0.0044(4) Uani 1 12 d S
Rh4 Rh 0.5000 0.0000 0.0000 0.0049(2) Uani 1 4 d S
O1 O 0.6660(6) 0.0000 0.0791(5) 0.0064(13) Uani 1 2 d S
O2 O 1.1680(6) 0.0000 0.0796(5) 0.0078(14) Uani 1 2 d S
O3 O 0.4914(5) 0.1570(5) 0.0838(4) 0.0063(10) Uani 1 1 d .
O4 O 0.8260(8) 0.4815(8) 0.2500 0.0049(13) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rh Rh -1.1178 0.9187 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Pb1 O4 82.4(3) 9_765 .
O4 Pb1 O3 66.10(12) 9_765 7_655
O4 Pb1 O3 107.86(13) . 7_655
O4 Pb1 O3 107.86(13) 9_765 2_655
O4 Pb1 O3 66.10(12) . 2_655
O3 Pb1 O3 172.5(2) 7_655 2_655
O4 Pb1 O3 66.10(12) 9_765 22_655
O4 Pb1 O3 107.86(13) . 22_655
O3 Pb1 O3 114.1(2) 7_655 22_655
O3 Pb1 O3 65.4(2) 2_655 22_655
O4 Pb1 O3 107.86(13) 9_765 17_656
O4 Pb1 O3 66.10(12) . 17_656
O3 Pb1 O3 65.4(2) 7_655 17_656
O3 Pb1 O3 114.1(2) 2_655 17_656
O3 Pb1 O3 172.5(2) 22_655 17_656
O4 Pb1 Rh1 109.73(15) 9_765 .
O4 Pb1 Rh1 36.34(13) . .
O3 Pb1 Rh1 140.73(10) 7_655 .
O3 Pb1 Rh1 35.43(10) 2_655 .
O3 Pb1 Rh1 97.02(11) 22_655 .
O3 Pb1 Rh1 80.62(11) 17_656 .
O4 Pb1 Rh1 36.34(13) 9_765 7_655
O4 Pb1 Rh1 109.73(16) . 7_655
O3 Pb1 Rh1 35.43(10) 7_655 7_655
O3 Pb1 Rh1 140.73(11) 2_655 7_655
O3 Pb1 Rh1 80.62(11) 22_655 7_655
O3 Pb1 Rh1 97.02(11) 17_656 7_655
Rh1 Pb1 Rh1 143.76(2) . 7_655
O4 Pb1 Rh1 109.73(15) 9_765 16_556
O4 Pb1 Rh1 36.34(13) . 16_556
O3 Pb1 Rh1 97.02(11) 7_655 16_556
O3 Pb1 Rh1 80.62(11) 2_655 16_556
O3 Pb1 Rh1 140.73(10) 22_655 16_556
O3 Pb1 Rh1 35.43(10) 17_656 16_556
Rh1 Pb1 Rh1 45.72(5) . 16_556
Rh1 Pb1 Rh1 120.31(4) 7_655 16_556
O4 Pb1 Rh1 36.34(13) 9_765 22_655
O4 Pb1 Rh1 109.73(16) . 22_655
O3 Pb1 Rh1 80.62(11) 7_655 22_655
O3 Pb1 Rh1 97.02(11) 2_655 22_655
O3 Pb1 Rh1 35.43(10) 22_655 22_655
O3 Pb1 Rh1 140.73(11) 17_656 22_655
Rh1 Pb1 Rh1 120.31(4) . 22_655
Rh1 Pb1 Rh1 45.72(5) 7_655 22_655
Rh1 Pb1 Rh1 143.76(2) 16_556 22_655
O4 Pb1 Pb2 41.22(17) 9_765 2_655
O4 Pb1 Pb2 41.22(17) . 2_655
O3 Pb1 Pb2 86.25(10) 7_655 2_655
O3 Pb1 Pb2 86.25(10) 2_655 2_655
O3 Pb1 Pb2 86.25(10) 22_655 2_655
O3 Pb1 Pb2 86.25(10) 17_656 2_655
Rh1 Pb1 Pb2 71.878(11) . 2_655
Rh1 Pb1 Pb2 71.878(11) 7_655 2_655
Rh1 Pb1 Pb2 71.878(11) 16_556 2_655
Rh1 Pb1 Pb2 71.878(11) 22_655 2_655
O4 Pb1 Bi2 41.22(17) 9_765 2_655
O4 Pb1 Bi2 41.22(17) . 2_655
O3 Pb1 Bi2 86.25(10) 7_655 2_655
O3 Pb1 Bi2 86.25(10) 2_655 2_655
O3 Pb1 Bi2 86.25(10) 22_655 2_655
O3 Pb1 Bi2 86.25(10) 17_656 2_655
Rh1 Pb1 Bi2 71.878(11) . 2_655
Rh1 Pb1 Bi2 71.878(11) 7_655 2_655
Rh1 Pb1 Bi2 71.878(11) 16_556 2_655
Rh1 Pb1 Bi2 71.878(11) 22_655 2_655
Pb2 Pb1 Bi2 0.0 2_655 2_655
O4 Pb2 O4 83.9(3) 7_545 3_665
O4 Pb2 O1 76.81(12) 7_545 .
O4 Pb2 O1 76.81(12) 3_665 .
O4 Pb2 O1 76.81(12) 7_545 16_556
O4 Pb2 O1 76.81(12) 3_665 16_556
O1 Pb2 O1 144.2(3) . 16_556
O4 Pb2 Bi1 41.97(16) 7_545 3_665
O4 Pb2 Bi1 41.97(16) 3_665 3_665
O1 Pb2 Bi1 72.12(16) . 3_665
O1 Pb2 Bi1 72.12(16) 16_556 3_665
O4 Pb2 Pb1 41.97(16) 7_545 3_665
O4 Pb2 Pb1 41.97(16) 3_665 3_665
O1 Pb2 Pb1 72.12(16) . 3_665
O1 Pb2 Pb1 72.12(16) 16_556 3_665
Bi1 Pb2 Pb1 0.0 3_665 3_665
O4 Pb2 Pb1 142.80(16) 7_545 .
O4 Pb2 Pb1 58.86(16) 3_665 .
O1 Pb2 Pb1 93.31(3) . .
O1 Pb2 Pb1 93.31(3) 16_556 .
Bi1 Pb2 Pb1 100.830(12) 3_665 .
Pb1 Pb2 Pb1 100.830(12) 3_665 .
O4 Pb2 Bi1 58.86(16) 7_545 2_645
O4 Pb2 Bi1 142.80(16) 3_665 2_645
O1 Pb2 Bi1 93.31(3) . 2_645
O1 Pb2 Bi1 93.31(3) 16_556 2_645
Bi1 Pb2 Bi1 100.830(12) 3_665 2_645
Pb1 Pb2 Bi1 100.830(12) 3_665 2_645
Pb1 Pb2 Bi1 158.34(2) . 2_645
O4 Pb2 Pb1 58.86(16) 7_545 2_645
O4 Pb2 Pb1 142.80(16) 3_665 2_645
O1 Pb2 Pb1 93.31(3) . 2_645
O1 Pb2 Pb1 93.31(3) 16_556 2_645
Bi1 Pb2 Pb1 100.830(12) 3_665 2_645
Pb1 Pb2 Pb1 100.830(12) 3_665 2_645
Pb1 Pb2 Pb1 158.34(2) . 2_645
Bi1 Pb2 Pb1 0.000(13) 2_645 2_645
O3 Rh1 O3 103.45(17) 2_655 .
O3 Rh1 O3 103.45(17) 2_655 3_665
O3 Rh1 O3 103.45(17) . 3_665
O3 Rh1 O4 88.1(2) 2_655 3_665
O3 Rh1 O4 83.4(2) . 3_665
O3 Rh1 O4 164.6(2) 3_665 3_665
O3 Rh1 O4 83.4(2) 2_655 .
O3 Rh1 O4 164.6(2) . .
O3 Rh1 O4 88.1(2) 3_665 .
O4 Rh1 O4 83.11(19) 3_665 .
O3 Rh1 O4 164.6(2) 2_655 2_655
O3 Rh1 O4 88.1(2) . 2_655
O3 Rh1 O4 83.4(2) 3_665 2_655
O4 Rh1 O4 83.11(19) 3_665 2_655
O4 Rh1 O4 83.11(19) . 2_655
O3 Rh1 Rh1 114.98(15) 2_655 16_556
O3 Rh1 Rh1 114.98(15) . 16_556
O3 Rh1 Rh1 114.98(15) 3_665 16_556
O4 Rh1 Rh1 49.99(13) 3_665 16_556
O4 Rh1 Rh1 49.99(13) . 16_556
O4 Rh1 Rh1 49.99(13) 2_655 16_556
O3 Rh1 Pb1 48.81(15) 2_655 .
O3 Rh1 Pb1 134.47(14) . .
O3 Rh1 Pb1 116.76(13) 3_665 .
O4 Rh1 Pb1 63.52(18) 3_665 .
O4 Rh1 Pb1 42.37(18) . .
O4 Rh1 Pb1 115.81(14) 2_655 .
Rh1 Rh1 Pb1 67.14(3) 16_556 .
O3 Rh1 Pb1 116.76(13) 2_655 3_665
O3 Rh1 Pb1 48.81(15) . 3_665
O3 Rh1 Pb1 134.47(14) 3_665 3_665
O4 Rh1 Pb1 42.37(18) 3_665 3_665
O4 Rh1 Pb1 115.81(14) . 3_665
O4 Rh1 Pb1 63.52(18) 2_655 3_665
Rh1 Rh1 Pb1 67.14(3) 16_556 3_665
Pb1 Rh1 Pb1 105.88(3) . 3_665
O3 Rh1 Bi1 116.76(13) 2_655 3_665
O3 Rh1 Bi1 48.81(15) . 3_665
O3 Rh1 Bi1 134.47(14) 3_665 3_665
O4 Rh1 Bi1 42.37(18) 3_665 3_665
O4 Rh1 Bi1 115.81(14) . 3_665
O4 Rh1 Bi1 63.52(18) 2_655 3_665
Rh1 Rh1 Bi1 67.14(3) 16_556 3_665
Pb1 Rh1 Bi1 105.88(3) . 3_665
Pb1 Rh1 Bi1 0.00(2) 3_665 3_665
O3 Rh1 Pb1 134.47(14) 2_655 2_655
O3 Rh1 Pb1 116.76(13) . 2_655
O3 Rh1 Pb1 48.81(15) 3_665 2_655
O4 Rh1 Pb1 115.81(14) 3_665 2_655
O4 Rh1 Pb1 63.52(18) . 2_655
O4 Rh1 Pb1 42.37(18) 2_655 2_655
Rh1 Rh1 Pb1 67.14(3) 16_556 2_655
Pb1 Rh1 Pb1 105.88(3) . 2_655
Pb1 Rh1 Pb1 105.88(3) 3_665 2_655
Bi1 Rh1 Pb1 105.88(3) 3_665 2_655
O3 Rh2 O3 91.6(3) 24_655 13_655
O3 Rh2 O1 84.1(2) 24_655 15_545
O3 Rh2 O1 96.6(2) 13_655 15_545
O3 Rh2 O1 96.6(2) 24_655 .
O3 Rh2 O1 84.1(2) 13_655 .
O1 Rh2 O1 179.0(3) 15_545 .
O3 Rh2 O2 92.1(2) 24_655 3_765
O3 Rh2 O2 176.3(2) 13_655 3_765
O1 Rh2 O2 83.8(2) 15_545 3_765
O1 Rh2 O2 95.4(2) . 3_765
O3 Rh2 O2 176.3(2) 24_655 13_755
O3 Rh2 O2 92.1(2) 13_655 13_755
O1 Rh2 O2 95.4(2) 15_545 13_755
O1 Rh2 O2 83.8(2) . 13_755
O2 Rh2 O2 84.2(4) 3_765 13_755
O3 Rh2 Rh4 41.97(14) 24_655 3_655
O3 Rh2 Rh4 93.14(14) 13_655 3_655
O1 Rh2 Rh4 42.23(19) 15_545 3_655
O1 Rh2 Rh4 138.51(14) . 3_655
O2 Rh2 Rh4 89.66(16) 3_765 3_655
O2 Rh2 Rh4 137.65(14) 13_755 3_655
O3 Rh2 Rh4 93.14(14) 24_655 .
O3 Rh2 Rh4 41.97(14) 13_655 .
O1 Rh2 Rh4 138.51(14) 15_545 .
O1 Rh2 Rh4 42.23(19) . .
O2 Rh2 Rh4 137.65(14) 3_765 .
O2 Rh2 Rh4 89.66(16) 13_755 .
Rh4 Rh2 Rh4 120.78(2) 3_655 .
O3 Rh2 Rh3 134.18(14) 24_655 .
O3 Rh2 Rh3 134.18(14) 13_655 .
O1 Rh2 Rh3 89.50(17) 15_545 .
O1 Rh2 Rh3 89.50(17) . .
O2 Rh2 Rh3 42.11(19) 3_765 .
O2 Rh2 Rh3 42.11(19) 13_755 .
Rh4 Rh2 Rh3 119.612(12) 3_655 .
Rh4 Rh2 Rh3 119.612(12) . .
O3 Rh2 Rh2 138.25(14) 24_655 14_665
O3 Rh2 Rh2 87.19(13) 13_655 14_665
O1 Rh2 Rh2 137.52(19) 15_545 14_665
O1 Rh2 Rh2 41.73(14) . 14_665
O2 Rh2 Rh2 90.01(16) 3_765 14_665
O2 Rh2 Rh2 42.10(14) 13_755 14_665
Rh4 Rh2 Rh2 179.612(12) 3_655 14_665
Rh4 Rh2 Rh2 59.612(12) . 14_665
Rh3 Rh2 Rh2 60.0 . 14_665
O3 Rh2 Rh2 87.19(13) 24_655 15_545
O3 Rh2 Rh2 138.25(14) 13_655 15_545
O1 Rh2 Rh2 41.73(14) 15_545 15_545
O1 Rh2 Rh2 137.52(19) . 15_545
O2 Rh2 Rh2 42.10(14) 3_765 15_545
O2 Rh2 Rh2 90.01(16) 13_755 15_545
Rh4 Rh2 Rh2 59.612(12) 3_655 15_545
Rh4 Rh2 Rh2 179.612(12) . 15_545
Rh3 Rh2 Rh2 60.0 . 15_545
Rh2 Rh2 Rh2 120.0 14_665 15_545
O2 Rh3 O2 84.2(3) 14_665 .
O2 Rh3 O2 84.2(3) 14_665 3_765
O2 Rh3 O2 95.8(3) . 3_765
O2 Rh3 O2 95.8(3) 14_665 13_755
O2 Rh3 O2 180.0(4) . 13_755
O2 Rh3 O2 84.2(3) 3_765 13_755
O2 Rh3 O2 180.0(4) 14_665 2_645
O2 Rh3 O2 95.8(3) . 2_645
O2 Rh3 O2 95.8(3) 3_765 2_645
O2 Rh3 O2 84.2(3) 13_755 2_645
O2 Rh3 O2 95.8(3) 14_665 15_545
O2 Rh3 O2 84.2(3) . 15_545
O2 Rh3 O2 180.0(3) 3_765 15_545
O2 Rh3 O2 95.8(3) 13_755 15_545
O2 Rh3 O2 84.2(3) 2_645 15_545
O2 Rh3 Rh2 90.0 14_665 13_755
O2 Rh3 Rh2 42.10(13) . 13_755
O2 Rh3 Rh2 137.90(13) 3_765 13_755
O2 Rh3 Rh2 137.90(13) 13_755 13_755
O2 Rh3 Rh2 90.0 2_645 13_755
O2 Rh3 Rh2 42.10(13) 15_545 13_755
O2 Rh3 Rh2 42.10(13) 14_665 15_545
O2 Rh3 Rh2 90.0 . 15_545
O2 Rh3 Rh2 42.10(13) 3_765 15_545
O2 Rh3 Rh2 90.0 13_755 15_545
O2 Rh3 Rh2 137.90(13) 2_645 15_545
O2 Rh3 Rh2 137.90(13) 15_545 15_545
Rh2 Rh3 Rh2 120.0 13_755 15_545
O2 Rh3 Rh2 90.0 14_665 .
O2 Rh3 Rh2 137.90(13) . .
O2 Rh3 Rh2 42.10(13) 3_765 .
O2 Rh3 Rh2 42.10(13) 13_755 .
O2 Rh3 Rh2 90.0 2_645 .
O2 Rh3 Rh2 137.90(13) 15_545 .
Rh2 Rh3 Rh2 180.000(16) 13_755 .
Rh2 Rh3 Rh2 60.0 15_545 .
O2 Rh3 Rh2 137.90(13) 14_665 3_765
O2 Rh3 Rh2 90.0 . 3_765
O2 Rh3 Rh2 137.90(13) 3_765 3_765
O2 Rh3 Rh2 90.0 13_755 3_765
O2 Rh3 Rh2 42.10(13) 2_645 3_765
O2 Rh3 Rh2 42.10(13) 15_545 3_765
Rh2 Rh3 Rh2 60.0 13_755 3_765
Rh2 Rh3 Rh2 180.0 15_545 3_765
Rh2 Rh3 Rh2 120.0 . 3_765
O2 Rh3 Rh2 42.10(13) 14_665 2_645
O2 Rh3 Rh2 42.10(13) . 2_645
O2 Rh3 Rh2 90.0 3_765 2_645
O2 Rh3 Rh2 137.90(13) 13_755 2_645
O2 Rh3 Rh2 137.90(13) 2_645 2_645
O2 Rh3 Rh2 90.0 15_545 2_645
Rh2 Rh3 Rh2 60.0 13_755 2_645
Rh2 Rh3 Rh2 60.0 15_545 2_645
Rh2 Rh3 Rh2 120.0 . 2_645
Rh2 Rh3 Rh2 120.0 3_765 2_645
O2 Rh3 Rh2 137.90(13) 14_665 14_665
O2 Rh3 Rh2 137.90(13) . 14_665
O2 Rh3 Rh2 90.0 3_765 14_665
O2 Rh3 Rh2 42.10(13) 13_755 14_665
O2 Rh3 Rh2 42.10(13) 2_645 14_665
O2 Rh3 Rh2 90.0 15_545 14_665
Rh2 Rh3 Rh2 120.0 13_755 14_665
Rh2 Rh3 Rh2 120.0 15_545 14_665
Rh2 Rh3 Rh2 60.0 . 14_665
Rh2 Rh3 Rh2 60.0 3_765 14_665
Rh2 Rh3 Rh2 180.000(8) 2_645 14_665
O3 Rh4 O3 180.0(3) 13_655 .
O3 Rh4 O3 90.7(3) 13_655 23
O3 Rh4 O3 89.3(3) . 23
O3 Rh4 O3 89.3(3) 13_655 11_655
O3 Rh4 O3 90.7(3) . 11_655
O3 Rh4 O3 180.0(2) 23 11_655
O3 Rh4 O1 84.27(19) 13_655 .
O3 Rh4 O1 95.73(19) . .
O3 Rh4 O1 95.73(19) 23 .
O3 Rh4 O1 84.27(19) 11_655 .
O3 Rh4 O1 95.73(19) 13_655 13_655
O3 Rh4 O1 84.27(19) . 13_655
O3 Rh4 O1 84.27(19) 23 13_655
O3 Rh4 O1 95.73(19) 11_655 13_655
O1 Rh4 O1 180.0(4) . 13_655
O3 Rh4 Rh2 88.13(13) 13_655 14_665
O3 Rh4 Rh2 91.87(13) . 14_665
O3 Rh4 Rh2 138.07(14) 23 14_665
O3 Rh4 Rh2 41.93(14) 11_655 14_665
O1 Rh4 Rh2 42.45(13) . 14_665
O1 Rh4 Rh2 137.55(13) 13_655 14_665
O3 Rh4 Rh2 91.87(13) 13_655 2_545
O3 Rh4 Rh2 88.13(13) . 2_545
O3 Rh4 Rh2 41.93(14) 23 2_545
O3 Rh4 Rh2 138.07(14) 11_655 2_545
O1 Rh4 Rh2 137.55(13) . 2_545
O1 Rh4 Rh2 42.45(13) 13_655 2_545
Rh2 Rh4 Rh2 180.0 14_665 2_545
O3 Rh4 Rh2 41.93(14) 13_655 .
O3 Rh4 Rh2 138.07(14) . .
O3 Rh4 Rh2 91.87(13) 23 .
O3 Rh4 Rh2 88.13(13) 11_655 .
O1 Rh4 Rh2 42.45(13) . .
O1 Rh4 Rh2 137.55(13) 13_655 .
Rh2 Rh4 Rh2 60.78(2) 14_665 .
Rh2 Rh4 Rh2 119.22(2) 2_545 .
O3 Rh4 Rh2 138.07(14) 13_655 13_655
O3 Rh4 Rh2 41.93(14) . 13_655
O3 Rh4 Rh2 88.13(13) 23 13_655
O3 Rh4 Rh2 91.87(13) 11_655 13_655
O1 Rh4 Rh2 137.55(13) . 13_655
O1 Rh4 Rh2 42.45(13) 13_655 13_655
Rh2 Rh4 Rh2 119.22(2) 14_665 13_655
Rh2 Rh4 Rh2 60.78(2) 2_545 13_655
Rh2 Rh4 Rh2 180.000(17) . 13_655
Rh4 O1 Rh2 95.3(2) . 14_665
Rh4 O1 Rh2 95.3(2) . .
Rh2 O1 Rh2 96.5(3) 14_665 .
Rh4 O1 Pb2 139.1(3) . .
Rh2 O1 Pb2 111.2(2) 14_665 .
Rh2 O1 Pb2 111.2(2) . .
Rh2 O2 Rh2 95.8(3) 2_645 13_755
Rh2 O2 Rh3 95.8(2) 2_645 .
Rh2 O2 Rh3 95.8(2) 13_755 .
Rh2 O3 Rh4 96.1(2) 13_655 .
Rh2 O3 Rh1 124.6(2) 13_655 .
Rh4 O3 Rh1 125.7(2) . .
Rh2 O3 Pb1 115.7(2) 13_655 3_665
Rh4 O3 Pb1 96.41(19) . 3_665
Rh1 O3 Pb1 95.77(19) . 3_665
Rh2 O3 Bi1 115.7(2) 13_655 3_665
Rh4 O3 Bi1 96.41(19) . 3_665
Rh1 O3 Bi1 95.77(19) . 3_665
Rh1 O4 Rh1 80.0(3) . 16_556
Rh1 O4 Bi2 135.40(18) . 2_655
Rh1 O4 Bi2 135.40(18) 16_556 2_655
Rh1 O4 Pb2 135.40(18) . 2_655
Rh1 O4 Pb2 135.40(18) 16_556 2_655
Rh1 O4 Pb1 101.3(2) . .
Rh1 O4 Pb1 101.3(2) 16_556 .
Bi2 O4 Pb1 96.8(2) 2_655 .
Pb2 O4 Pb1 96.8(2) 2_655 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Pb1 O4 2.367(7) 9_765
Pb1 O4 2.367(7) .
Pb1 O3 2.605(5) 7_655
Pb1 O3 2.605(5) 2_655
Pb1 O3 2.605(5) 22_655
Pb1 O3 2.605(5) 17_656
Pb1 Rh1 3.4449(15) .
Pb1 Rh1 3.4449(15) 7_655
Pb1 Rh1 3.4449(15) 16_556
Pb1 Rh1 3.4449(15) 22_655
Pb1 Pb2 3.5151(19) 2_655
Pb1 Bi2 3.5151(19) 2_655
Pb2 O4 2.333(7) 7_545
Pb2 O4 2.333(7) 3_665
Pb2 O1 2.361(7) .
Pb2 O1 2.361(7) 16_556
Pb2 Bi1 3.5151(19) 3_665
Pb2 Pb1 3.5151(19) 3_665
Pb2 Bi1 3.6185(18) 2_645
Pb2 Pb1 3.6185(18) 2_645
Rh1 O3 2.007(5) 2_655
Rh1 O3 2.007(5) .
Rh1 O3 2.007(5) 3_665
Rh1 O4 2.082(5) 3_665
Rh1 O4 2.082(5) .
Rh1 O4 2.082(5) 2_655
Rh1 Rh1 2.677(3) 16_556
Rh1 Pb1 3.4449(15) 3_665
Rh1 Bi1 3.4449(15) 3_665
Rh1 Pb1 3.4449(15) 2_655
Rh2 O3 2.000(5) 24_655
Rh2 O3 2.000(5) 13_655
Rh2 O1 2.017(4) 15_545
Rh2 O1 2.017(4) .
Rh2 O2 2.029(5) 3_765
Rh2 O2 2.029(5) 13_755
Rh2 Rh4 2.9764(15) 3_655
Rh2 Rh4 2.9764(15) .
Rh2 Rh3 3.0113(16) .
Rh2 Rh2 3.0113(16) 14_665
Rh2 Rh2 3.0113(16) 15_545
Rh3 O2 2.030(7) 14_665
Rh3 O2 2.030(7) .
Rh3 O2 2.030(7) 3_765
Rh3 O2 2.030(7) 13_755
Rh3 O2 2.030(7) 2_645
Rh3 O2 2.030(7) 15_545
Rh3 Rh2 3.0113(16) 13_755
Rh3 Rh2 3.0113(16) 15_545
Rh3 Rh2 3.0113(16) 3_765
Rh3 Rh2 3.0113(16) 2_645
Rh3 Rh2 3.0113(16) 14_665
Rh4 O3 2.002(5) 13_655
Rh4 O3 2.002(5) .
Rh4 O3 2.002(5) 23
Rh4 O3 2.002(5) 11_655
Rh4 O1 2.009(7) .
Rh4 O1 2.009(7) 13_655
Rh4 Rh2 2.9764(15) 14_665
Rh4 Rh2 2.9764(15) 2_545
Rh4 Rh2 2.9764(14) 13_655
O1 Rh2 2.017(4) 14_665
O2 Rh2 2.029(5) 2_645
O2 Rh2 2.029(5) 13_755
O3 Rh2 2.000(5) 13_655
O3 Pb1 2.605(5) 3_665
O3 Bi1 2.605(5) 3_665
O4 Rh1 2.082(5) 16_556
O4 Bi2 2.333(7) 2_655
O4 Pb2 2.333(7) 2_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O4 Pb1 Pb2 O4 0.0 . 7_545
O3 Pb1 Pb2 O4 113.57(12) 7_655 7_545
O3 Pb1 Pb2 O4 -61.71(11) 2_655 7_545
O3 Pb1 Pb2 O4 -113.57(12) 22_655 7_545
O3 Pb1 Pb2 O4 61.71(11) 17_656 7_545
Rh1 Pb1 Pb2 O4 -24.32(3) . 7_545
Rh1 Pb1 Pb2 O4 139.38(4) 7_655 7_545
Rh1 Pb1 Pb2 O4 24.32(3) 16_556 7_545
Rh1 Pb1 Pb2 O4 -139.38(4) 22_655 7_545
Pb2 Pb1 Pb2 O4 0.0 2_655 7_545
Bi2 Pb1 Pb2 O4 0.0 2_655 7_545
O4 Pb1 Pb2 O4 0.0 . 3_665
O3 Pb1 Pb2 O4 113.57(12) 7_655 3_665
O3 Pb1 Pb2 O4 -61.71(11) 2_655 3_665
O3 Pb1 Pb2 O4 -113.57(12) 22_655 3_665
O3 Pb1 Pb2 O4 61.71(11) 17_656 3_665
Rh1 Pb1 Pb2 O4 -24.32(3) . 3_665
Rh1 Pb1 Pb2 O4 139.38(4) 7_655 3_665
Rh1 Pb1 Pb2 O4 24.32(3) 16_556 3_665
Rh1 Pb1 Pb2 O4 -139.38(4) 22_655 3_665
Pb2 Pb1 Pb2 O4 0.0 2_655 3_665
Bi2 Pb1 Pb2 O4 0.0 2_655 3_665
O4 Pb1 Pb2 O1 72.42(16) . .
O3 Pb1 Pb2 O1 -174.01(19) 7_655 .
O3 Pb1 Pb2 O1 10.71(19) 2_655 .
O3 Pb1 Pb2 O1 -41.1(2) 22_655 .
O3 Pb1 Pb2 O1 134.1(2) 17_656 .
Rh1 Pb1 Pb2 O1 48.10(16) . .
Rh1 Pb1 Pb2 O1 -148.20(16) 7_655 .
Rh1 Pb1 Pb2 O1 96.74(16) 16_556 .
Rh1 Pb1 Pb2 O1 -66.96(17) 22_655 .
Pb2 Pb1 Pb2 O1 72.42(16) 2_655 .
Bi2 Pb1 Pb2 O1 72.42(16) 2_655 .
O4 Pb1 Pb2 O1 -72.42(16) . 16_556
O3 Pb1 Pb2 O1 41.1(2) 7_655 16_556
O3 Pb1 Pb2 O1 -134.1(2) 2_655 16_556
O3 Pb1 Pb2 O1 174.0(2) 22_655 16_556
O3 Pb1 Pb2 O1 -10.71(19) 17_656 16_556
Rh1 Pb1 Pb2 O1 -96.74(16) . 16_556
Rh1 Pb1 Pb2 O1 66.96(17) 7_655 16_556
Rh1 Pb1 Pb2 O1 -48.10(16) 16_556 16_556
Rh1 Pb1 Pb2 O1 148.20(16) 22_655 16_556
Pb2 Pb1 Pb2 O1 -72.42(16) 2_655 16_556
Bi2 Pb1 Pb2 O1 -72.42(16) 2_655 16_556
O4 Pb1 Pb2 Bi1 0.0 . 3_665
O3 Pb1 Pb2 Bi1 113.57(12) 7_655 3_665
O3 Pb1 Pb2 Bi1 -61.71(11) 2_655 3_665
O3 Pb1 Pb2 Bi1 -113.57(12) 22_655 3_665
O3 Pb1 Pb2 Bi1 61.71(11) 17_656 3_665
Rh1 Pb1 Pb2 Bi1 -24.32(3) . 3_665
Rh1 Pb1 Pb2 Bi1 139.38(4) 7_655 3_665
Rh1 Pb1 Pb2 Bi1 24.32(3) 16_556 3_665
Rh1 Pb1 Pb2 Bi1 -139.38(4) 22_655 3_665
Pb2 Pb1 Pb2 Bi1 0.0 2_655 3_665
Bi2 Pb1 Pb2 Bi1 0.0 2_655 3_665
O4 Pb1 Pb2 Pb1 0.0 . 3_665
O3 Pb1 Pb2 Pb1 113.57(12) 7_655 3_665
O3 Pb1 Pb2 Pb1 -61.71(11) 2_655 3_665
O3 Pb1 Pb2 Pb1 -113.57(12) 22_655 3_665
O3 Pb1 Pb2 Pb1 61.71(11) 17_656 3_665
Rh1 Pb1 Pb2 Pb1 -24.32(3) . 3_665
Rh1 Pb1 Pb2 Pb1 139.38(4) 7_655 3_665
Rh1 Pb1 Pb2 Pb1 24.32(3) 16_556 3_665
Rh1 Pb1 Pb2 Pb1 -139.38(4) 22_655 3_665
Pb2 Pb1 Pb2 Pb1 0.0 2_655 3_665
Bi2 Pb1 Pb2 Pb1 0.0 2_655 3_665
O3 Pb1 Pb2 Bi1 -66.43(12) 7_655 2_645
O3 Pb1 Pb2 Bi1 118.29(11) 2_655 2_645
O3 Pb1 Pb2 Bi1 66.43(12) 22_655 2_645
O3 Pb1 Pb2 Bi1 -118.29(11) 17_656 2_645
Rh1 Pb1 Pb2 Bi1 155.68(3) . 2_645
Rh1 Pb1 Pb2 Bi1 -40.62(4) 7_655 2_645
Rh1 Pb1 Pb2 Bi1 -155.68(3) 16_556 2_645
Rh1 Pb1 Pb2 Bi1 40.62(4) 22_655 2_645
Pb2 Pb1 Pb2 Bi1 180.0 2_655 2_645
Bi2 Pb1 Pb2 Bi1 180.0 2_655 2_645
O4 Pb1 Pb2 Pb1 180.0 . 2_645
O3 Pb1 Pb2 Pb1 -66.43(12) 7_655 2_645
O3 Pb1 Pb2 Pb1 118.29(11) 2_655 2_645
O3 Pb1 Pb2 Pb1 66.43(12) 22_655 2_645
O3 Pb1 Pb2 Pb1 -118.29(11) 17_656 2_645
Rh1 Pb1 Pb2 Pb1 155.68(3) . 2_645
Rh1 Pb1 Pb2 Pb1 -40.62(4) 7_655 2_645
Rh1 Pb1 Pb2 Pb1 -155.68(3) 16_556 2_645
Rh1 Pb1 Pb2 Pb1 40.62(4) 22_655 2_645
Pb2 Pb1 Pb2 Pb1 180.0 2_655 2_645
Bi2 Pb1 Pb2 Pb1 180.0 2_655 2_645
O4 Pb1 Rh1 O3 93.33(19) 9_765 2_655
O4 Pb1 Rh1 O3 137.0(3) . 2_655
O3 Pb1 Rh1 O3 169.4(3) 7_655 2_655
O3 Pb1 Rh1 O3 26.25(13) 22_655 2_655
O3 Pb1 Rh1 O3 -160.9(3) 17_656 2_655
Rh1 Pb1 Rh1 O3 109.96(18) 7_655 2_655
Rh1 Pb1 Rh1 O3 -167.98(18) 16_556 2_655
Rh1 Pb1 Rh1 O3 54.73(18) 22_655 2_655
Pb2 Pb1 Rh1 O3 109.96(18) 2_655 2_655
Bi2 Pb1 Rh1 O3 109.96(18) 2_655 2_655
O4 Pb1 Rh1 O3 158.1(2) 9_765 .
O4 Pb1 Rh1 O3 -158.2(3) . .
O3 Pb1 Rh1 O3 -125.9(3) 7_655 .
O3 Pb1 Rh1 O3 64.8(2) 2_655 .
O3 Pb1 Rh1 O3 91.0(2) 22_655 .
O3 Pb1 Rh1 O3 -96.2(3) 17_656 .
Rh1 Pb1 Rh1 O3 174.7(2) 7_655 .
Rh1 Pb1 Rh1 O3 -103.2(2) 16_556 .
Rh1 Pb1 Rh1 O3 119.5(2) 22_655 .
Pb2 Pb1 Rh1 O3 174.7(2) 2_655 .
Bi2 Pb1 Rh1 O3 174.7(2) 2_655 .
O4 Pb1 Rh1 O3 8.80(18) 9_765 3_665
O4 Pb1 Rh1 O3 52.5(2) . 3_665
O3 Pb1 Rh1 O3 84.8(2) 7_655 3_665
O3 Pb1 Rh1 O3 -84.5(2) 2_655 3_665
O3 Pb1 Rh1 O3 -58.28(18) 22_655 3_665
O3 Pb1 Rh1 O3 114.5(2) 17_656 3_665
Rh1 Pb1 Rh1 O3 25.43(16) 7_655 3_665
Rh1 Pb1 Rh1 O3 107.50(16) 16_556 3_665
Rh1 Pb1 Rh1 O3 -29.80(17) 22_655 3_665
Pb2 Pb1 Rh1 O3 25.43(16) 2_655 3_665
Bi2 Pb1 Rh1 O3 25.43(16) 2_655 3_665
O4 Pb1 Rh1 O4 -153.98(7) 9_765 3_665
O4 Pb1 Rh1 O4 -110.3(3) . 3_665
O3 Pb1 Rh1 O4 -78.0(2) 7_655 3_665
O3 Pb1 Rh1 O4 112.7(2) 2_655 3_665
O3 Pb1 Rh1 O4 138.94(17) 22_655 3_665
O3 Pb1 Rh1 O4 -48.26(18) 17_656 3_665
Rh1 Pb1 Rh1 O4 -137.36(14) 7_655 3_665
Rh1 Pb1 Rh1 O4 -55.29(14) 16_556 3_665
Rh1 Pb1 Rh1 O4 167.42(14) 22_655 3_665
Pb2 Pb1 Rh1 O4 -137.36(14) 2_655 3_665
Bi2 Pb1 Rh1 O4 -137.36(14) 2_655 3_665
O4 Pb1 Rh1 O4 -43.7(3) 9_765 .
O3 Pb1 Rh1 O4 32.4(2) 7_655 .
O3 Pb1 Rh1 O4 -137.0(3) 2_655 .
O3 Pb1 Rh1 O4 -110.7(2) 22_655 .
O3 Pb1 Rh1 O4 62.1(2) 17_656 .
Rh1 Pb1 Rh1 O4 -27.03(19) 7_655 .
Rh1 Pb1 Rh1 O4 55.03(19) 16_556 .
Rh1 Pb1 Rh1 O4 -82.3(2) 22_655 .
Pb2 Pb1 Rh1 O4 -27.03(19) 2_655 .
Bi2 Pb1 Rh1 O4 -27.03(19) 2_655 .
O4 Pb1 Rh1 O4 -86.9(2) 9_765 2_655
O4 Pb1 Rh1 O4 -43.3(3) . 2_655
O3 Pb1 Rh1 O4 -10.9(3) 7_655 2_655
O3 Pb1 Rh1 O4 179.7(3) 2_655 2_655
O3 Pb1 Rh1 O4 -154.0(2) 22_655 2_655
O3 Pb1 Rh1 O4 18.8(2) 17_656 2_655
Rh1 Pb1 Rh1 O4 -70.3(2) 7_655 2_655
Rh1 Pb1 Rh1 O4 11.8(2) 16_556 2_655
Rh1 Pb1 Rh1 O4 -125.5(2) 22_655 2_655
Pb2 Pb1 Rh1 O4 -70.3(2) 2_655 2_655
Bi2 Pb1 Rh1 O4 -70.3(2) 2_655 2_655
O4 Pb1 Rh1 Rh1 -98.70(7) 9_765 16_556
O4 Pb1 Rh1 Rh1 -55.03(19) . 16_556
O3 Pb1 Rh1 Rh1 -22.67(16) 7_655 16_556
O3 Pb1 Rh1 Rh1 167.98(18) 2_655 16_556
O3 Pb1 Rh1 Rh1 -165.77(10) 22_655 16_556
O3 Pb1 Rh1 Rh1 7.03(10) 17_656 16_556
Rh1 Pb1 Rh1 Rh1 -82.068(9) 7_655 16_556
Rh1 Pb1 Rh1 Rh1 -137.29(4) 22_655 16_556
Pb2 Pb1 Rh1 Rh1 -82.068(9) 2_655 16_556
Bi2 Pb1 Rh1 Rh1 -82.068(9) 2_655 16_556
O4 Pb1 Rh1 Pb1 -154.76(8) 9_765 3_665
O4 Pb1 Rh1 Pb1 -111.10(19) . 3_665
O3 Pb1 Rh1 Pb1 -78.73(16) 7_655 3_665
O3 Pb1 Rh1 Pb1 111.91(18) 2_655 3_665
O3 Pb1 Rh1 Pb1 138.16(10) 22_655 3_665
O3 Pb1 Rh1 Pb1 -49.03(11) 17_656 3_665
Rh1 Pb1 Rh1 Pb1 -138.13(4) 7_655 3_665
Rh1 Pb1 Rh1 Pb1 -56.06(3) 16_556 3_665
Rh1 Pb1 Rh1 Pb1 166.646(17) 22_655 3_665
Pb2 Pb1 Rh1 Pb1 -138.13(4) 2_655 3_665
Bi2 Pb1 Rh1 Pb1 -138.13(4) 2_655 3_665
O4 Pb1 Rh1 Bi1 -154.76(8) 9_765 3_665
O4 Pb1 Rh1 Bi1 -111.10(19) . 3_665
O3 Pb1 Rh1 Bi1 -78.73(16) 7_655 3_665
O3 Pb1 Rh1 Bi1 111.91(18) 2_655 3_665
O3 Pb1 Rh1 Bi1 138.16(10) 22_655 3_665
O3 Pb1 Rh1 Bi1 -49.03(11) 17_656 3_665
Rh1 Pb1 Rh1 Bi1 -138.13(4) 7_655 3_665
Rh1 Pb1 Rh1 Bi1 -56.06(3) 16_556 3_665
Rh1 Pb1 Rh1 Bi1 166.646(17) 22_655 3_665
Pb2 Pb1 Rh1 Bi1 -138.13(4) 2_655 3_665
Bi2 Pb1 Rh1 Bi1 -138.13(4) 2_655 3_665
O4 Pb1 Rh1 Pb1 -42.63(8) 9_765 2_655
O4 Pb1 Rh1 Pb1 1.03(19) . 2_655
O3 Pb1 Rh1 Pb1 33.40(16) 7_655 2_655
O3 Pb1 Rh1 Pb1 -135.96(18) 2_655 2_655
O3 Pb1 Rh1 Pb1 -109.71(11) 22_655 2_655
O3 Pb1 Rh1 Pb1 63.09(11) 17_656 2_655
Rh1 Pb1 Rh1 Pb1 -26.01(2) 7_655 2_655
Rh1 Pb1 Rh1 Pb1 56.06(3) 16_556 2_655
Rh1 Pb1 Rh1 Pb1 -81.23(6) 22_655 2_655
Pb2 Pb1 Rh1 Pb1 -26.01(2) 2_655 2_655
Bi2 Pb1 Rh1 Pb1 -26.01(2) 2_655 2_655
O3 Rh2 Rh3 O2 81.2(3) 24_655 14_665
O3 Rh2 Rh3 O2 -98.8(3) 13_655 14_665
O1 Rh2 Rh3 O2 0.0(3) 15_545 14_665
O1 Rh2 Rh3 O2 180.0(3) . 14_665
O2 Rh2 Rh3 O2 81.3(4) 3_765 14_665
O2 Rh2 Rh3 O2 -98.7(4) 13_755 14_665
Rh4 Rh2 Rh3 O2 31.0(2) 3_655 14_665
Rh4 Rh2 Rh3 O2 -149.0(2) . 14_665
Rh2 Rh2 Rh3 O2 -149.0(2) 14_665 14_665
Rh2 Rh2 Rh3 O2 31.0(2) 15_545 14_665
O3 Rh2 Rh3 O2 -0.1(3) 24_655 .
O3 Rh2 Rh3 O2 179.9(3) 13_655 .
O1 Rh2 Rh3 O2 -81.3(3) 15_545 .
O1 Rh2 Rh3 O2 98.7(3) . .
O2 Rh2 Rh3 O2 0.0 3_765 .
O2 Rh2 Rh3 O2 180.0 13_755 .
Rh4 Rh2 Rh3 O2 -50.3(2) 3_655 .
Rh4 Rh2 Rh3 O2 129.7(2) . .
Rh2 Rh2 Rh3 O2 129.7(2) 14_665 .
Rh2 Rh2 Rh3 O2 -50.3(2) 15_545 .
O3 Rh2 Rh3 O2 -0.1(3) 24_655 3_765
O3 Rh2 Rh3 O2 179.9(3) 13_655 3_765
O1 Rh2 Rh3 O2 -81.3(3) 15_545 3_765
O1 Rh2 Rh3 O2 98.7(3) . 3_765
O2 Rh2 Rh3 O2 180.0 13_755 3_765
Rh4 Rh2 Rh3 O2 -50.3(2) 3_655 3_765
Rh4 Rh2 Rh3 O2 129.7(2) . 3_765
Rh2 Rh2 Rh3 O2 129.7(2) 14_665 3_765
Rh2 Rh2 Rh3 O2 -50.3(2) 15_545 3_765
O3 Rh2 Rh3 O2 179.9(3) 24_655 13_755
O3 Rh2 Rh3 O2 -0.1(3) 13_655 13_755
O1 Rh2 Rh3 O2 98.7(3) 15_545 13_755
O1 Rh2 Rh3 O2 -81.3(3) . 13_755
O2 Rh2 Rh3 O2 180.0 3_765 13_755
Rh4 Rh2 Rh3 O2 129.7(2) 3_655 13_755
Rh4 Rh2 Rh3 O2 -50.3(2) . 13_755
Rh2 Rh2 Rh3 O2 -50.3(2) 14_665 13_755
Rh2 Rh2 Rh3 O2 129.7(2) 15_545 13_755
O3 Rh2 Rh3 O2 -98.8(3) 24_655 2_645
O3 Rh2 Rh3 O2 81.2(3) 13_655 2_645
O1 Rh2 Rh3 O2 180.0(3) 15_545 2_645
O1 Rh2 Rh3 O2 0.0(3) . 2_645
O2 Rh2 Rh3 O2 -98.7(4) 3_765 2_645
O2 Rh2 Rh3 O2 81.3(4) 13_755 2_645
Rh4 Rh2 Rh3 O2 -149.0(2) 3_655 2_645
Rh4 Rh2 Rh3 O2 31.0(2) . 2_645
Rh2 Rh2 Rh3 O2 31.0(2) 14_665 2_645
Rh2 Rh2 Rh3 O2 -149.0(2) 15_545 2_645
O3 Rh2 Rh3 O2 179.9(3) 24_655 15_545
O3 Rh2 Rh3 O2 -0.1(3) 13_655 15_545
O1 Rh2 Rh3 O2 98.7(3) 15_545 15_545
O1 Rh2 Rh3 O2 -81.3(3) . 15_545
O2 Rh2 Rh3 O2 180.0 3_765 15_545
O2 Rh2 Rh3 O2 0.0 13_755 15_545
Rh4 Rh2 Rh3 O2 129.7(2) 3_655 15_545
Rh4 Rh2 Rh3 O2 -50.3(2) . 15_545
Rh2 Rh2 Rh3 O2 -50.3(2) 14_665 15_545
Rh2 Rh2 Rh3 O2 129.7(2) 15_545 15_545
O3 Rh2 Rh3 Rh2 50.20(19) 24_655 15_545
O3 Rh2 Rh3 Rh2 -129.80(19) 13_655 15_545
O1 Rh2 Rh3 Rh2 -31.05(18) 15_545 15_545
O1 Rh2 Rh3 Rh2 148.95(18) . 15_545
O1 Rh2 Rh3 Rh2 -31.05(18) . 3_765
O1 Rh2 Rh3 Rh2 -31.05(18) 15_545 2_645
O1 Rh2 Rh3 Rh2 148.95(18) . 2_645
O2 Rh2 Rh3 Rh2 50.3(2) 3_765 2_645
O2 Rh2 Rh3 Rh2 -129.7(2) 13_755 2_645
Rh4 Rh2 Rh3 Rh2 0.0 3_655 2_645
Rh4 Rh2 Rh3 Rh2 180.0 . 2_645
Rh2 Rh2 Rh3 Rh2 180.0 14_665 2_645
Rh2 Rh2 Rh3 Rh2 0.0 15_545 2_645
O3 Rh2 Rh3 Rh2 -129.80(19) 24_655 14_665
O3 Rh2 Rh3 Rh2 50.20(19) 13_655 14_665
O1 Rh2 Rh3 Rh2 148.95(18) 15_545 14_665
O1 Rh2 Rh3 Rh2 -31.05(18) . 14_665
O2 Rh2 Rh3 Rh2 -129.7(2) 3_765 14_665
O2 Rh2 Rh3 Rh2 50.3(2) 13_755 14_665
Rh4 Rh2 Rh3 Rh2 180.0 3_655 14_665
Rh4 Rh2 Rh3 Rh2 0.0 . 14_665
Rh2 Rh2 Rh3 Rh2 180.0 15_545 14_665
O3 Rh2 Rh4 O3 -89.0(3) 24_655 13_655
O1 Rh2 Rh4 O3 -4.3(4) 15_545 13_655
O1 Rh2 Rh4 O3 174.6(3) . 13_655
O2 Rh2 Rh4 O3 174.5(4) 3_765 13_655
O2 Rh2 Rh4 O3 93.5(3) 13_755 13_655
Rh4 Rh2 Rh4 O3 -55.5(2) 3_655 13_655
Rh3 Rh2 Rh4 O3 124.5(2) . 13_655
O3 Rh2 Rh4 O3 91.0(3) 24_655 .
O3 Rh2 Rh4 O3 180.0 13_655 .
O1 Rh2 Rh4 O3 175.7(4) 15_545 .
O1 Rh2 Rh4 O3 -5.4(3) . .
O2 Rh2 Rh4 O3 -5.5(4) 3_765 .
O2 Rh2 Rh4 O3 -86.5(3) 13_755 .
Rh4 Rh2 Rh4 O3 124.5(2) 3_655 .
Rh3 Rh2 Rh4 O3 -55.5(2) . .
Rh2 Rh2 Rh4 O3 -55.5(2) 14_665 .
O3 Rh2 Rh4 O3 -0.07(13) 24_655 23
O3 Rh2 Rh4 O3 88.9(3) 13_655 23
O1 Rh2 Rh4 O3 84.6(3) 15_545 23
O1 Rh2 Rh4 O3 -96.5(3) . 23
O2 Rh2 Rh4 O3 -96.6(3) 3_765 23
O2 Rh2 Rh4 O3 -177.6(2) 13_755 23
Rh4 Rh2 Rh4 O3 33.42(15) 3_655 23
Rh3 Rh2 Rh4 O3 -146.58(15) . 23
O3 Rh2 Rh4 O3 179.93(13) 24_655 11_655
O3 Rh2 Rh4 O3 -91.1(3) 13_655 11_655
O1 Rh2 Rh4 O3 -95.4(3) 15_545 11_655
O1 Rh2 Rh4 O3 83.5(3) . 11_655
O2 Rh2 Rh4 O3 83.4(3) 3_765 11_655
O2 Rh2 Rh4 O3 2.4(2) 13_755 11_655
Rh4 Rh2 Rh4 O3 -146.58(15) 3_655 11_655
Rh3 Rh2 Rh4 O3 33.42(15) . 11_655
O3 Rh2 Rh4 O1 96.4(3) 24_655 .
O3 Rh2 Rh4 O1 -174.6(3) 13_655 .
O1 Rh2 Rh4 O1 -179.0(3) 15_545 .
O2 Rh2 Rh4 O1 -0.2(4) 3_765 .
O2 Rh2 Rh4 O1 -81.2(3) 13_755 .
Rh3 Rh2 Rh4 O1 -50.1(2) . .
Rh2 Rh2 Rh4 O1 -50.1(2) 14_665 .
O3 Rh2 Rh4 O1 -83.6(3) 24_655 13_655
O3 Rh2 Rh4 O1 5.4(3) 13_655 13_655
O1 Rh2 Rh4 O1 1.0(3) 15_545 13_655
O1 Rh2 Rh4 O1 180.0 . 13_655
O2 Rh2 Rh4 O1 179.8(4) 3_765 13_655
O2 Rh2 Rh4 O1 98.8(3) 13_755 13_655
Rh4 Rh2 Rh4 O1 -50.1(2) 3_655 13_655
Rh3 Rh2 Rh4 O1 129.9(2) . 13_655
O3 Rh2 Rh4 Rh2 -124.5(2) 13_655 14_665
O2 Rh2 Rh4 Rh2 50.0(3) 3_765 14_665
O3 Rh2 Rh4 Rh2 -33.49(14) 24_655 2_545
O3 Rh2 Rh4 Rh2 55.5(2) 13_655 2_545
O1 Rh2 Rh4 Rh2 51.1(3) 15_545 2_545
O1 Rh2 Rh4 Rh2 -129.9(2) . 2_545
O2 Rh2 Rh4 Rh2 -130.0(3) 3_765 2_545
O2 Rh2 Rh4 Rh2 148.95(18) 13_755 2_545
Rh4 Rh2 Rh4 Rh2 0.0 3_655 2_545
O3 Rh4 O1 Rh2 93.5(2) 13_655 14_665
O3 Rh4 O1 Rh2 -86.5(2) . 14_665
O3 Rh4 O1 Rh2 -176.4(2) 23 14_665
O3 Rh4 O1 Rh2 3.6(2) 11_655 14_665
Rh2 Rh4 O1 Rh2 180.0 2_545 14_665
Rh2 Rh4 O1 Rh2 97.1(3) . 14_665
Rh2 Rh4 O1 Rh2 -82.9(3) 13_655 14_665
O3 Rh4 O1 Rh2 -3.6(2) 13_655 .
O3 Rh4 O1 Rh2 176.4(2) . .
O3 Rh4 O1 Rh2 86.5(2) 23 .
O3 Rh4 O1 Rh2 -93.5(2) 11_655 .
Rh2 Rh4 O1 Rh2 -97.1(3) 14_665 .
Rh2 Rh4 O1 Rh2 82.9(3) 2_545 .
Rh2 Rh4 O1 Rh2 180.0 13_655 .
O3 Rh4 O1 Pb2 -135.04(14) 13_655 .
O3 Rh4 O1 Pb2 44.96(14) . .
O3 Rh4 O1 Pb2 -44.96(14) 23 .
O3 Rh4 O1 Pb2 135.04(14) 11_655 .
Rh2 Rh4 O1 Pb2 131.45(16) 14_665 .
Rh2 Rh4 O1 Pb2 -48.55(16) 2_545 .
Rh2 Rh4 O1 Pb2 -131.45(16) . .
Rh2 Rh4 O1 Pb2 48.55(16) 13_655 .
O3 Rh2 O1 Rh4 -87.4(2) 24_655 .
O3 Rh2 O1 Rh4 3.6(2) 13_655 .
O2 Rh2 O1 Rh4 179.9(2) 3_765 .
O2 Rh2 O1 Rh4 96.3(3) 13_755 .
Rh4 Rh2 O1 Rh4 -84.5(3) 3_655 .
Rh3 Rh2 O1 Rh4 138.15(16) . .
Rh2 Rh2 O1 Rh4 96.0(3) 14_665 .
Rh2 Rh2 O1 Rh4 179.559(14) 15_545 .
O3 Rh2 O1 Rh2 176.6(2) 24_655 14_665
O3 Rh2 O1 Rh2 -92.4(3) 13_655 14_665
O2 Rh2 O1 Rh2 83.9(3) 3_765 14_665
O2 Rh2 O1 Rh2 0.3(3) 13_755 14_665
Rh4 Rh2 O1 Rh2 179.546(15) 3_655 14_665
Rh4 Rh2 O1 Rh2 -96.0(3) . 14_665
Rh3 Rh2 O1 Rh2 42.2(2) . 14_665
Rh2 Rh2 O1 Rh2 83.6(3) 15_545 14_665
O3 Rh2 O1 Pb2 60.8(3) 24_655 .
O3 Rh2 O1 Pb2 151.8(2) 13_655 .
O2 Rh2 O1 Pb2 -31.9(3) 3_765 .
O2 Rh2 O1 Pb2 -115.5(3) 13_755 .
Rh4 Rh2 O1 Pb2 63.8(4) 3_655 .
Rh4 Rh2 O1 Pb2 148.2(3) . .
Rh3 Rh2 O1 Pb2 -73.6(2) . .
Rh2 Rh2 O1 Pb2 -115.8(4) 14_665 .
Rh2 Rh2 O1 Pb2 -32.2(3) 15_545 .
O4 Pb2 O1 Rh4 43.38(16) 7_545 .
O4 Pb2 O1 Rh4 -43.38(16) 3_665 .
O1 Pb2 O1 Rh4 0.0 16_556 .
Bi1 Pb2 O1 Rh4 0.0 3_665 .
Pb1 Pb2 O1 Rh4 0.0 3_665 .
Pb1 Pb2 O1 Rh4 -100.318(15) . .
Bi1 Pb2 O1 Rh4 100.318(15) 2_645 .
Pb1 Pb2 O1 Rh4 100.318(15) 2_645 .
O4 Pb2 O1 Rh2 170.2(3) 7_545 14_665
O4 Pb2 O1 Rh2 83.4(2) 3_665 14_665
O1 Pb2 O1 Rh2 126.8(2) 16_556 14_665
Bi1 Pb2 O1 Rh2 126.8(2) 3_665 14_665
Pb1 Pb2 O1 Rh2 126.8(2) 3_665 14_665
Pb1 Pb2 O1 Rh2 26.5(2) . 14_665
Bi1 Pb2 O1 Rh2 -132.9(2) 2_645 14_665
Pb1 Pb2 O1 Rh2 -132.9(2) 2_645 14_665
O4 Pb2 O1 Rh2 -83.4(2) 7_545 .
O4 Pb2 O1 Rh2 -170.2(3) 3_665 .
O1 Pb2 O1 Rh2 -126.8(2) 16_556 .
Bi1 Pb2 O1 Rh2 -126.8(2) 3_665 .
Pb1 Pb2 O1 Rh2 -126.8(2) 3_665 .
Pb1 Pb2 O1 Rh2 132.9(2) . .
Bi1 Pb2 O1 Rh2 -26.5(2) 2_645 .
Pb1 Pb2 O1 Rh2 -26.5(2) 2_645 .
O2 Rh3 O2 Rh2 0.0 14_665 2_645
O2 Rh3 O2 Rh2 83.5(3) 3_765 2_645
O2 Rh3 O2 Rh2 180.0 2_645 2_645
O2 Rh3 O2 Rh2 -96.5(3) 15_545 2_645
Rh2 Rh3 O2 Rh2 -96.5(3) 13_755 2_645
Rh2 Rh3 O2 Rh2 41.77(16) 15_545 2_645
Rh2 Rh3 O2 Rh2 83.5(3) . 2_645
Rh2 Rh3 O2 Rh2 -138.23(16) 3_765 2_645
Rh2 Rh3 O2 Rh2 180.0 14_665 2_645
O2 Rh3 O2 Rh2 96.5(3) 14_665 13_755
O2 Rh3 O2 Rh2 180.0 3_765 13_755
O2 Rh3 O2 Rh2 -83.5(3) 2_645 13_755
O2 Rh3 O2 Rh2 0.0 15_545 13_755
Rh2 Rh3 O2 Rh2 138.23(16) 15_545 13_755
Rh2 Rh3 O2 Rh2 180.0 . 13_755
Rh2 Rh3 O2 Rh2 -41.77(16) 3_765 13_755
Rh2 Rh3 O2 Rh2 96.5(3) 2_645 13_755
Rh2 Rh3 O2 Rh2 -83.5(3) 14_665 13_755
O3 Rh4 O3 Rh2 -87.9(2) 23 13_655
O3 Rh4 O3 Rh2 92.1(2) 11_655 13_655
O1 Rh4 O3 Rh2 176.4(2) . 13_655
O1 Rh4 O3 Rh2 -3.6(2) 13_655 13_655
Rh2 Rh4 O3 Rh2 134.00(15) 14_665 13_655
Rh2 Rh4 O3 Rh2 -46.00(15) 2_545 13_655
Rh2 Rh4 O3 Rh2 180.0 . 13_655
O3 Rh4 O3 Rh1 130.8(2) 23 .
O3 Rh4 O3 Rh1 -49.2(2) 11_655 .
O1 Rh4 O3 Rh1 35.1(3) . .
O1 Rh4 O3 Rh1 -144.9(3) 13_655 .
Rh2 Rh4 O3 Rh1 -7.3(3) 14_665 .
Rh2 Rh4 O3 Rh1 172.7(3) 2_545 .
Rh2 Rh4 O3 Rh1 38.7(4) . .
Rh2 Rh4 O3 Rh1 -141.3(4) 13_655 .
O3 Rh4 O3 Pb1 28.9(2) 23 3_665
O3 Rh4 O3 Pb1 -151.1(2) 11_655 3_665
O1 Rh4 O3 Pb1 -66.79(18) . 3_665
O1 Rh4 O3 Pb1 113.21(18) 13_655 3_665
Rh2 Rh4 O3 Pb1 -109.16(11) 14_665 3_665
Rh2 Rh4 O3 Pb1 70.84(11) 2_545 3_665
Rh2 Rh4 O3 Pb1 -63.2(2) . 3_665
Rh2 Rh4 O3 Pb1 116.8(2) 13_655 3_665
O3 Rh4 O3 Bi1 28.9(2) 23 3_665
O3 Rh4 O3 Bi1 -151.1(2) 11_655 3_665
O1 Rh4 O3 Bi1 -66.79(18) . 3_665
O1 Rh4 O3 Bi1 113.21(18) 13_655 3_665
Rh2 Rh4 O3 Bi1 -109.16(11) 14_665 3_665
Rh2 Rh4 O3 Bi1 70.84(11) 2_545 3_665
Rh2 Rh4 O3 Bi1 -63.2(2) . 3_665
Rh2 Rh4 O3 Bi1 116.8(2) 13_655 3_665
O3 Rh1 O3 Rh2 -119.17(12) 2_655 13_655
O3 Rh1 O3 Rh2 -11.5(4) 3_665 13_655
O4 Rh1 O3 Rh2 154.4(3) 3_665 13_655
O4 Rh1 O3 Rh2 126.0(8) . 13_655
O4 Rh1 O3 Rh2 71.2(3) 2_655 13_655
Rh1 Rh1 O3 Rh2 114.6(3) 16_556 13_655
Pb1 Rh1 O3 Rh2 -163.59(14) . 13_655
Pb1 Rh1 O3 Rh2 126.9(3) 3_665 13_655
Bi1 Rh1 O3 Rh2 126.9(3) 3_665 13_655
Pb1 Rh1 O3 Rh2 38.8(3) 2_655 13_655
O3 Rh1 O3 Rh4 11.8(4) 2_655 .
O3 Rh1 O3 Rh4 119.42(13) 3_665 .
O4 Rh1 O3 Rh4 -74.6(3) 3_665 .
O4 Rh1 O3 Rh4 -103.1(8) . .
O4 Rh1 O3 Rh4 -157.9(3) 2_655 .
Rh1 Rh1 O3 Rh4 -114.4(3) 16_556 .
Pb1 Rh1 O3 Rh4 -32.6(4) . .
Pb1 Rh1 O3 Rh4 -102.2(3) 3_665 .
Bi1 Rh1 O3 Rh4 -102.2(3) 3_665 .
Pb1 Rh1 O3 Rh4 169.8(2) 2_655 .
O3 Rh1 O3 Pb1 114.0(2) 2_655 3_665
O3 Rh1 O3 Pb1 -138.4(2) 3_665 3_665
O4 Rh1 O3 Pb1 27.57(19) 3_665 3_665
O4 Rh1 O3 Pb1 -0.9(9) . 3_665
O4 Rh1 O3 Pb1 -55.72(19) 2_655 3_665
Rh1 Rh1 O3 Pb1 -12.23(18) 16_556 3_665
Pb1 Rh1 O3 Pb1 69.5(2) . 3_665
Bi1 Rh1 O3 Pb1 0.0 3_665 3_665
Pb1 Rh1 O3 Pb1 -88.04(14) 2_655 3_665
O3 Rh1 O3 Bi1 114.0(2) 2_655 3_665
O3 Rh1 O3 Bi1 -138.4(2) 3_665 3_665
O4 Rh1 O3 Bi1 27.57(19) 3_665 3_665
O4 Rh1 O3 Bi1 -0.9(9) . 3_665
O4 Rh1 O3 Bi1 -55.72(19) 2_655 3_665
Rh1 Rh1 O3 Bi1 -12.23(18) 16_556 3_665
Pb1 Rh1 O3 Bi1 69.5(2) . 3_665
Pb1 Rh1 O3 Bi1 0.0 3_665 3_665
Pb1 Rh1 O3 Bi1 -88.04(14) 2_655 3_665
O3 Rh1 O4 Rh1 -130.8(2) 2_655 16_556
O3 Rh1 O4 Rh1 -13.4(9) . 16_556
O3 Rh1 O4 Rh1 125.5(2) 3_665 16_556
O4 Rh1 O4 Rh1 -41.92(8) 3_665 16_556
O4 Rh1 O4 Rh1 41.92(8) 2_655 16_556
Pb1 Rh1 O4 Rh1 -99.6(2) . 16_556
Pb1 Rh1 O4 Rh1 -14.2(2) 3_665 16_556
Bi1 Rh1 O4 Rh1 -14.2(2) 3_665 16_556
Pb1 Rh1 O4 Rh1 81.46(15) 2_655 16_556
O3 Rh1 O4 Bi2 80.9(4) 2_655 2_655
O3 Rh1 O4 Bi2 -161.8(6) . 2_655
O3 Rh1 O4 Bi2 -22.9(4) 3_665 2_655
O4 Rh1 O4 Bi2 169.7(5) 3_665 2_655
O4 Rh1 O4 Bi2 -106.4(5) 2_655 2_655
Rh1 Rh1 O4 Bi2 -148.3(5) 16_556 2_655
Pb1 Rh1 O4 Bi2 112.0(4) . 2_655
Pb1 Rh1 O4 Bi2 -162.5(3) 3_665 2_655
Bi1 Rh1 O4 Bi2 -162.5(3) 3_665 2_655
Pb1 Rh1 O4 Bi2 -66.9(4) 2_655 2_655
O3 Rh1 O4 Pb2 80.9(4) 2_655 2_655
O3 Rh1 O4 Pb2 -161.8(6) . 2_655
O3 Rh1 O4 Pb2 -22.9(4) 3_665 2_655
O4 Rh1 O4 Pb2 169.7(5) 3_665 2_655
O4 Rh1 O4 Pb2 -106.4(5) 2_655 2_655
Rh1 Rh1 O4 Pb2 -148.3(5) 16_556 2_655
Pb1 Rh1 O4 Pb2 112.0(4) . 2_655
Pb1 Rh1 O4 Pb2 -162.5(3) 3_665 2_655
Bi1 Rh1 O4 Pb2 -162.5(3) 3_665 2_655
Pb1 Rh1 O4 Pb2 -66.9(4) 2_655 2_655
O3 Rh1 O4 Pb1 -31.11(19) 2_655 .
O3 Rh1 O4 Pb1 86.2(8) . .
O3 Rh1 O4 Pb1 -134.9(2) 3_665 .
O4 Rh1 O4 Pb1 57.7(3) 3_665 .
O4 Rh1 O4 Pb1 141.6(2) 2_655 .
Rh1 Rh1 O4 Pb1 99.6(2) 16_556 .
Pb1 Rh1 O4 Pb1 85.45(15) 3_665 .
Bi1 Rh1 O4 Pb1 85.45(15) 3_665 .
Pb1 Rh1 O4 Pb1 -178.9(2) 2_655 .
O4 Pb1 O4 Rh1 139.04(15) 9_765 .
O3 Pb1 O4 Rh1 -159.14(14) 7_655 .
O3 Pb1 O4 Rh1 25.63(14) 2_655 .
O3 Pb1 O4 Rh1 77.2(2) 22_655 .
O3 Pb1 O4 Rh1 -107.6(3) 17_656 .
Rh1 Pb1 O4 Rh1 163.41(13) 7_655 .
Rh1 Pb1 O4 Rh1 -81.9(3) 16_556 .
Rh1 Pb1 O4 Rh1 114.66(19) 22_655 .
Pb2 Pb1 O4 Rh1 139.04(15) 2_655 .
Bi2 Pb1 O4 Rh1 139.04(15) 2_655 .
O4 Pb1 O4 Rh1 -139.04(15) 9_765 16_556
O3 Pb1 O4 Rh1 -77.2(2) 7_655 16_556
O3 Pb1 O4 Rh1 107.6(3) 2_655 16_556
O3 Pb1 O4 Rh1 159.14(14) 22_655 16_556
O3 Pb1 O4 Rh1 -25.63(14) 17_656 16_556
Rh1 Pb1 O4 Rh1 81.9(3) . 16_556
Rh1 Pb1 O4 Rh1 -114.66(19) 7_655 16_556
Rh1 Pb1 O4 Rh1 -163.41(13) 22_655 16_556
Pb2 Pb1 O4 Rh1 -139.04(15) 2_655 16_556
Bi2 Pb1 O4 Rh1 -139.04(15) 2_655 16_556
O4 Pb1 O4 Bi2 0.0 9_765 2_655
O3 Pb1 O4 Bi2 61.82(12) 7_655 2_655
O3 Pb1 O4 Bi2 -113.41(13) 2_655 2_655
O3 Pb1 O4 Bi2 -61.82(12) 22_655 2_655
O3 Pb1 O4 Bi2 113.41(13) 17_656 2_655
Rh1 Pb1 O4 Bi2 -139.04(15) . 2_655
Rh1 Pb1 O4 Bi2 24.38(4) 7_655 2_655
Rh1 Pb1 O4 Bi2 139.04(15) 16_556 2_655
Rh1 Pb1 O4 Bi2 -24.38(4) 22_655 2_655
Pb2 Pb1 O4 Bi2 0.0 2_655 2_655
O4 Pb1 O4 Pb2 0.0 9_765 2_655
O3 Pb1 O4 Pb2 61.82(12) 7_655 2_655
O3 Pb1 O4 Pb2 -113.41(13) 2_655 2_655
O3 Pb1 O4 Pb2 -61.82(12) 22_655 2_655
O3 Pb1 O4 Pb2 113.41(13) 17_656 2_655
Rh1 Pb1 O4 Pb2 -139.04(15) . 2_655
Rh1 Pb1 O4 Pb2 24.38(4) 7_655 2_655
Rh1 Pb1 O4 Pb2 139.04(15) 16_556 2_655
Rh1 Pb1 O4 Pb2 -24.38(4) 22_655 2_655
Bi2 Pb1 O4 Pb2 0.0 2_655 2_655
